| ||Format||Pages||Price|| |
|7||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||7||$50.00||  ADD TO CART|
Significance and Use
3.1 These methods determine the compressive strength of structural panels in response to stresses acting in the plane of the panel.
3.2 Method A—This method is applicable to structural panels of uniform properties within a panel. It is useful for evaluating plywood of clear, straight-grained veneers, and determining the effect of chemical or preservative treatments, construction, principal direction with respect to direction of stress, and other variables that are expected to uniformly influence the panel.
3.3 Method B:
3.3.1 The compressive properties obtained by this method are a reliable approximation of the strength of a full-size panel, and are intended for use in design.
3.3.2 The compressive properties are influenced by buckling; however, this effect can be eliminated in this test by restraining the edges of the specimens.
3.4 It is recommended that where comparisons are to be made, that the same method and specimen size be used throughout. This is because the volume of material included in a test specimen can influence the compressive strength regardless of whether the material properties are uniform throughout the sheet or vary widely due to the presence of growth or manufacturing features.
1.1 These test methods cover the determination of the compression properties of wood-based structural panels. Wood-based structural panels in use include plywood, waferboard, oriented strand board, and composites of veneer and of wood-based layers.
1.2 Method A, Compression Test for Small Specimens—This method is applicable to small specimens that are uniform with respect to elastic and strength properties. Two types of compression tests are employed: one to evaluate both elastic and compressive strength properties, and the second to evaluate maximum compressive strength only.
1.3 Method B, Compression Test for Large Specimens—This method employs large specimens and responds well to manufacturing variables and growth characteristics that influence compression properties of structural panels.
1.3.1 This method is intended for the following:
22.214.171.124 Comparative tests of structural panels,
126.96.36.199 Evaluating the effects of moisture content on strength properties of structural panels,
188.8.131.52 Determining the strength properties of structural panels, and
184.108.40.206 Evaluating the effects of raw material and manufacturing variables on compression properties of structural panels.
1.4 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D2395 Test Methods for Density and Specific Gravity (Relative Density) of Wood and Wood-Based Materials
D4442 Test Methods for Direct Moisture Content Measurement of Wood and Wood-Based Materials
ICS Number Code 79.060.10 (Plywood)
UNSPSC Code 11121600(Wood)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D3501-05a(2018), Standard Test Methods for Wood-Based Structural Panels in Compression, ASTM International, West Conshohocken, PA, 2018, www.astm.orgBack to Top